SOLUTIONS TO PROBLEMS

PREFACE

This section of instructors materials contains solutions and answers to all

problems and questions that appear in the textbook. My penmanship leaves

something to be desired; therefore, I generated these solutions/answers using

computer software so that the resulting product would be "readable." Furthermore, I

endeavored to provide complete and detailed solutions in order that: (1) the

instructor, without having to take time to solve a problem, will understand what

principles/skills are to be learned by its solution; and (2) to facilitate student

understanding/learning when the solution is posted.

I would recommended that the course instructor consult these

solutions/answers before assigning problems and questions. In doing so, he or she

ensures that the students will be drilled in the intended principles and concepts. In

addition, the instructor may provide appropriate hints for some of the more difficult

problems.

With regard to symbols, in the text material I elected to boldface those symbols

that are italicized in the textbook. Furthermore, I also endeavored to be consistent

relative to symbol style. However, in several instances, symbols that appear in the

textbook were not available, and it was necessary to make appropriate substitutions.

These include the following: the letter a (unit cell edge length, crack length) is used in

place of the cursive a. And Roman F and E replace script F (Faraday's constant in

Chapter 18) and script E (electric field in Chapter 19), respectively.

I have exercised extreme care in designing these problems/questions, and then

in solving them. However, no matter how careful one is with the preparation of a work

such as this, errors will always remain in the final product. Therefore, corrections,

suggestions, and comments from instructors who use the textbook (as well as their

teaching assistants) pertaining to homework problems/solutions are welcomed. These

may be sent to me in care of the publisher.

CHAPTER 2

ATOMIC STRUCTURE AND INTERATOMIC BONDING

PROBLEM SOLUTIONS

2.1 (a) When two or more atoms of an element have different atomic masses, each is termed an

isotope.

(b) The atomic weights of the elements ordinarily are not integers because: (1) the atomic

12

masses of the atoms generally are not integers (except for

C), and (2) the atomic weight is

taken as the weighted average of the atomic masses of an atom's naturally occurring isotopes.

2.2

Atomic mass is the mass of an individual atom, whereas atomic weight is the average

(weighted) of the atomic masses of an atom's naturally occurring isotopes.

2.3 (a) In order to determine the number of grams in one amu of material, appropriate manipulation

of the amu/atom, g/mol, and atom/mol relationships is all that is necessary, as

#g/amu =

1 mol

1 g/mol

6.023 x 1023 atoms 1 amu/atom

(

)

= 1.66 x 10-24 g/amu

(b) Since there are 453.6 g/lbm ,

1 lb-mol = (453.6 g/lbm )(6.023 x 1023 atoms/g-mol)

= 2.73 x 1026 atoms/lb-mol

2.4 (a) Two important quantum-mechanical concepts associated with the Bohr model of the atom

are that electrons are particles moving in discrete orbitals, and electron energy is quantized into

shells.

(b)

Two important refinements resulting from the wave-mechanical atomic model are that

electron position is described in terms of a probability distribution, and electron energy is

quantized into both shells and subshells--each electron is characterized by four quantum

numbers.

1

2.5 The n quantum number designates the electron shell.

The l quantum number designates the electron subshell.

The m quantum number designates the number of electron states in each electron subshell.

l

The m quantum number designates the spin moment on each electron.

s

2.6 For the L state, n = 2, and eight electron states are possible. Possible l values are 0 and 1,

while possible m l values are 0 and ±1. Therefore, for the s states, the quantum numbers are

1

1

1

1

1

200( ) and 200(- ). For the p states, the quantum numbers are 210( ), 210(- ), 211( ), 211(2

2

2

2

2

1

1

1

), 21(-1)( ), and 21(-1)(- ).

2

2

2

For the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2;

1

possible m l values are 0, ±1, and ±2; and possible m s values are ± . Therefore, for the s

2

1

1

1

1

states, the quantum numbers are 300( ), 300(- ), for the p states they are 310( ), 310(- ),

2

2

2

2

311(\F(1,2)), 311(-\F(1,2)), 31(-1)(\F(1,2)), and 31(-1)(-\F(1,2)); for the d states they are

1

1

1

1

1

1

1

1

1

1

320( ), 320(- ), 321( ), 321(- ), 32(-1)( ), 32(-1)(- ), 322( ), 322(- ), 32(-2)( ), and 32(-2)(- ).

2

2

2

2

2

2

2

2

2

2

2.7 The electron configurations of the ions are determined using Table 2.2.

2 2 6 2 6 6

- 1s 2s 2p 3s 3p 3d

3+

2 2 6 2 6 5

Fe

- 1s 2s 2p 3s 3p 3d

+

2 2 6 2 6 10

Cu - 1s 2s 2p 3s 3p 3d

2+

2 2 6 2 6 10 2 6 10 2 6

Ba

- 1s 2s 2p 3s 3p 3d 4s 4p 4d 5s 5p

2 2 6 2 6 10 2 6

Br - 1s 2s 2p 3s 3p 3d 4s 4p

22 2 6 2 6

S - 1s 2s 2p 3s 3p

Fe

2.8 The Cs

+

2+

ion is just a cesium atom that has lost one electron; therefore, it has an electron

configuration the same as xenon (Figure 2.6).

The Br ion is a bromine atom that has acquired one extra electron; therefore, it has an

electron configuration the same as krypton.

2.9 Each of the elements in Group VIIA has five p electrons.

2 2 6 2 6 7 2

2.10 (a) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because

of an incomplete d subshell.

2

2 2 6 2 6

(b) The 1s 2s 2p 3s 3p electron configuration is that of an inert gas because of filled 3s and

3p subshells.

2 2 5

(c) The 1s 2s 2p electron configuration is that of a halogen because it is one electron

deficient from having a filled L shell.

2 2 6 2

(d) The 1s 2s 2p 3s electron configuration is that of an alkaline earth metal because of two s

electrons.

2 2 6 2 6 2 2

(e) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of

an incomplete d subshell.

2 2 6 2 6 1

(f) The 1s 2s 2p 3s 3p 4s electron configuration is that of an alkali metal because of a

single s electron.

2.11 (a) The 4f subshell is being filled for the rare earth series of elements.

(b) The 5f subshell is being filled for the actinide series of elements.

2.12 The attractive force between two ions F A is just the derivative with respect to the interatomic

separation of the attractive energy expression, Equation (2.8), which is just

FA =

dEA

dr

( Ar) = A

d =

dr

r2

The constant A in this expression is defined in footnote 3 on page 21. Since the valences of

the K+ and O2- ions are +1 and -2, respectively, Z1 = 1 and Z 2 = 2, then

FA =

=

(Z1e)(Z2e)

4πε o r2

(1)(2)(1.6 x 10-19 C)2

(4)(π)(8.85 x 10-12 F/m)(1.5 x 10-9 m)2

= 2.05 x 10-10 N

2.13 (a) Differentiation of Equation (2.11) yields

dEN

dr

A

nB

= (1 + 1) - (n + 1) = 0

r

r

3

(b) Now, solving for r (= r )

o

A

nB

= (n + 1)

2

ro ro

or

ro =

(nBA )

1/(1 - n)

(c) Substitution for ro into Equation (2.11) and solving for E (= Eo)

A B

+

ro rn

o

Eo = -

=-

A

+

A 1/(1 - n)

nB

( )

B

A n/(1 - n)

nB

( )

2.14 (a) Curves of E , E , and E are shown on the plot below.

A R

N

2

1

E

R

0

Bonding Energy (eV)

EN

-1

r = 0.28 nm

o

-2

-3

-4

E o = -4.6 eV

-5

EA

-6

-7

0.0

0.2

0.4

0.6

Interatomic Separation (nm)

4

0.8

1.0

(b) From this plot

r = 0.28 nm

o

E = -4.6 eV

o

(c) From Equation (2.11) for E

N

A = 1.436

B = 5.86 x 10

-6

n=9

Thus,

ro =

=

(nBA )

1/(1 - n)

1.436

1/(1 - 9) = 0.279 nm

-6

(9)(5.86 x 10 )

and

Eo= -

1.436

5.86 x 10-6

+

1.436

1.436

1/(1 - 9)

9/(1 - 9)

-6

-6

(9)(5.86 x 10 )

(9)(5.86 x 10 )

= - 4.57 eV

2.15 This problem gives us, for a hypothetical X+ -Y- ion pair, values for ro (0.35 nm), E o (-6.13 eV),

and n (10), and asks that we determine explicit expressions for attractive and repulsive energies

of Equations 2.8 and 2.9. In essence, it is necessary to compute the values of A and B in

these equations. Expressions for r o and E o in terms of n, A , and B were determined in

Problem 2.13, which are as follows:

ro =

Eo = -

(nBA )

1/(1 - n)

A

+

A 1/(1 - n)

nB

( )

B

A n/(1 - n)

nB

( )

Thus, we have two simultaneous equations with two unknowns (viz. A and B). Upon substitution

of values for ro and E o in terms of n, these equations take the forms

5

A

(10B

)

0.35 nm =

-6.13 eV = -

1/(1 - 10)

A

+

A 1/(1 - 10)

10B

( )

B

A 10/(1 - 10)

10B

( )

Simultaneous solution of these two equations leads to A = 2.38 and B = 1.88 x 10-5 . Thus,

Equations (2.8) and (2.9) become

EA = -

ER =

2.38

r

1.88 x 10-5

r10

Of course these expressions are valid for r and E in units of nanometers and electron volts,

respectively.

2.16 (a) Differentiating Equation (2.12) with respect to r yields

dE C De-r/ρ

= dr r2

ρ

At r = ro , dE/dr = 0, and

C De-ro/ρ

2=

ρ

ro

Solving for C and substitution into Equation (2.12) yields an expression for E o as

r

Eo = De-ro/ρ 1 - o

ρ

(b) Now solving for D from Equation (2.12b) above yields

D=

r /ρ

Cρe o

r2o

6

(2.12b)

Substitution of this expression for D into Equation (2.12) yields an expression for Eo as

Eo =

C ρ

- 1

ro ro

2.17 (a) The main differences between the various forms of primary bonding are:

Ionic--there is electrostatic attraction between oppositely charged ions.

Covalent--there is electron sharing between two adjacent atoms such that each atom

assumes a stable electron configuration.

Metallic--the positively charged ion cores are shielded from one another, and also "glued"

together by the sea of valence electrons.

(b) The Pauli exclusion principle states that each electron state can hold no more than two

electrons, which must have opposite spins.

2.18 Covalently bonded materials are less dense than metallic or ionically bonded ones because

covalent bonds are directional in nature whereas metallic and ionic are not; when bonds are

directional, the atoms cannot pack together in as dense a manner, yielding a lower mass

density.

2.19 The percent ionic character is a function of the electron negativities of the ions X A and X B

according to Equation (2.10). The electronegativities of the elements are found in Figure 2.7.

For TiO2, X Ti = 1.5 and X O = 3.5, and therefore,

[

%IC = 1 - e(-0.25)(3.5 - 1.5)

2

] x 100 = 63.2%

For ZnTe, X Zn = 1.6 and X Te = 2.1, and therefore,

[

%IC = 1 - e(-0.25)(2.1 - 1.6)

2

] x 100 = 6.1%

For CsCl, X Cs = 0.7 and X Cl = 3.0, and therefore,

[

%IC = 1 - e(-0.25)(3.0 - 0.7)

For InSb, X In = 1.7 and X Sb = 1.9, and therefore,

7

2

] x 100 = 73.4%

[

%IC = 1 - e(-0.25)(1.9 - 1.7)

2

] x 100 = 1.0%

For MgCl2, X Mg = 1.2 and X Cl = 3.0, and therefore,

[

%IC = 1 - e(-0.25)(3.0 - 1.2)

2

] x 100 = 55.5%

2.20 Below is plotted the bonding energy versus melting temperature for these four metals. From

this plot, the bonding energy for copper (melting temperature of 1084°C) should be

approximately 3.6 eV. The experimental value is 3.5 eV.

Bonding Energy (eV)

10

W

8

6

4

Fe

3.6 eV

Al

2

0

-1000

Hg

0

1000

2000

3000

4000

Melting Temperature (C)

2 2

2.21 For germanium, having the valence electron structure 4s 4p , N' = 4; thus, there are 8 - N' = 4

covalent bonds per atom.

2 3

For phosphorus, having the valence electron structure 3s 3p , N' = 5; thus, there are 8

- N' = 3 covalent bonds per atom.

2 4

For selenium, having the valence electron structure 4s 4p , N' = 6; thus, there are 8 N' = 2 covalent bonds per atom.

2 5

For chlorine, having the valence electron structure 3s 3p , N' = 7; thus, there is 8 - N' =

1 covalent bond per atom.

2.22 For brass, the bonding is metallic since it is a metal alloy.

For rubber, the bonding is covalent with some van der Waals. (Rubber is composed

primarily of carbon and hydrogen atoms.)

8

For BaS, the bonding is predominantly ionic (but with some covalent character) on the

basis of the relative positions of Ba and S in the periodic table.

For solid xenon, the bonding is van der Waals since xenon is an inert gas.

For bronze, the bonding is metallic since it is a metal alloy (composed of copper and tin).

For nylon, the bonding is covalent with perhaps some van der Waals.

(Nylon is

composed primarily of carbon and hydrogen.)

For AlP the bonding is predominantly covalent (but with some ionic character) on the

basis of the relative positions of Al and P in the periodic table.

2.23 The intermolecular bonding for HF is hydrogen, whereas for HCl, the intermolecular bonding is

van der Waals. Since the hydrogen bond is stronger than van der Waals, HF will have a higher

melting temperature.

2.24 The geometry of the H O molecules, which are hydrogen bonded to one another, is more

2

restricted in the solid phase than for the liquid. This results in a more open molecular structure in

the solid, and a less dense solid phase.

9

CHAPTER 3

THE STRUCTURE OF CRYSTALLINE SOLIDS

PROBLEM SOLUTIONS

3.1 Atomic structure relates to the number of protons and neutrons in the nucleus of an atom, as

well as the number and probability distributions of the constituent electrons. On the other hand,

crystal structure pertains to the arrangement of atoms in the crystalline solid material.

3.2 A crystal structure is described by both the geometry of, and atomic arrangements within, the

unit cell, whereas a crystal system is described only in terms of the unit cell geometry. For

example, face-centered cubic and body-centered cubic are crystal structures that belong to the

cubic crystal system.

3.3 For this problem, we are asked to calculate the volume of a unit cell of aluminum. Aluminum

has an FCC crystal structure (Table 3.1). The FCC unit cell volume may be computed from

Equation (3.4) as

√ 2 = (16)(0.143 x 10-9 m)3√ 2 = 6.62 x 10-29 m3

VC = 16R3

3.4 This problem calls for a demonstration of the relationship a = 4R

√ 3 for BCC. Consider the BCC

unit cell shown below

a

Q

a

P

N

O

a

Using the triangle NOP

10

__

2

(NP) = a2 + a2 = 2a2

And then for triangle NPQ,

__

__

__

(NQ )2 = (QP )2 + (NP )2

__

__

But NQ = 4R, R being the atomic radius. Also, QP = a. Therefore,

(4R)2 = a2 + 2a2, or

a=

4R

3

√

3.5 We are asked to show that the ideal c/a ratio for HCP is 1.633. A sketch of one-third of an HCP

unit cell is shown below.

a

c

M

L

J

K

a

Consider the tetrahedron labeled as JKLM, which is reconstructed as

11

M

L

H

J

K

__

The atom at point M is midway between the top and bottom faces of the unit cell--that is M H =

c/2. And, since atoms at points J, K, and M, all touch one another,

__ __

JM = JK = 2R = a

where R is the atomic radius. Furthermore, from triangle JHM,

__

__

__

__

(c2)2

(JM )2 = ( JH )2 + (MH)2, or

a2 = ( JH )2 +

__

Now, we can determine the JH length by consideration of triangle JKL, which is an equilateral

triangle,

L

J

30

H

a/2

K

cos 30° =

a/2

√ 3 , and

=

JH

2

__

JH =

12

a

3

√

__

Substituting this value for JH in the above expression yields

a2 =

2

2

a 2 + c 2 = a + c

2

3

4

3

√

()

and, solving for c/a

c

=

a

√ 83 = 1.633

3.6 We are asked to show that the atomic packing factor for BCC is 0.68. The atomic packing factor

is defined as the ratio of sphere volume to the total unit cell volume, or

APF =

VS

VC

Since there are two spheres associated with each unit cell for BCC

4πR3 8πR 3

=

3

3

V S = 2(sphere volume) = 2

Also, the unit cell has cubic symmetry, that is V

C

3

= a . But a depends on R according to

Equation (3.3), and

VC =

4R 3

3

√

=

64R 3

3√

3

Thus,

APF =

8πR 3 /3

= 0.68

64R 3 /3

√3

3.7 This problem calls for a demonstration that the APF for HCP is 0.74. Again, the APF is just the

total sphere-unit cell volume ratio. For HCP, there are the equivalent of six spheres per unit cell,

and thus

13

4πR3

= 8πR 3

3

V S = 6

Now, the unit cell volume is just the product of the base area times the cell height, c. This base

area is just three times the area of the parallelepiped ACDE shown below.

D

C

a = 2R

30

60

E

A

B

a = 2R

a = 2R

__

__

__

The area of ACDE is just the length of CD times the height BC. But CD is just a or 2R, and

__

BC = 2R cos(30°) =

2R

√3

2

Thus, the base area is just

__ __

2R√ 3

= 6R2

√3

2

AREA = (3)(CD )(BC ) = (3)(2R)

and since c = 1.633a = 2R(1.633)

VC = (AREA)(c) = 6R2c

√ 3 = (6R2√ 3)(2)(1.633)R = 12√ 3(1.633)R3

Thus,

APF =

VS

VC

=

8πR 3

12 √

3(1.633)R3

= 0.74

3.8 This problem calls for a computation of the density of iron. According to Equation (3.5)

14

ρ=

nAFe

VCNA

For BCC, n = 2 atoms/unit cell, and

VC =

4R 3

3

√

Thus,

ρ=

(2 atoms/unit cell)(55.9 g/mol)

(4)(0.124 x 10-7 cm)3/

√ 3 3/(unit cell)(6.023 x 1023 atoms/mol)

[

]

= 7.90 g/cm3

3

The value given inside the front cover is 7.87 g/cm .

3.9 We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal

structure. For FCC, n = 4 atoms/unit cell, and V = 16R3

√ 2 [Equation (3.4)]. Now,

C

ρ=

nAIr

VCNA

And solving for R from the above two expressions yields

16ρNA√ 2

R=

nAIr

1/3

(4 atoms/unit cell)(192.2 g/mol)

=

3

23

(√ 2)(16)(22.4 g/cm )(6.023 x 10 atoms/mol)

1/3

= 1.36 x 10-8 cm = 0.136 nm

3.10

This problem asks for us to calculate the radius of a vanadium atom. For BCC, n = 2

atoms/unit cell, and

15

VC =

4R 3

3

√

=

64R 3

3√

3

Since,

ρ=

nA V

VCNA

and solving for R

R=

3√

3nA V 1/3

64ρNA

(3√ 3)(2 atoms/unit cell)(50.9 g/mol) 1/3

=

(64)(5.96 g/cm3)(6.023 x 1023 atoms/mol)

= 1.32 x 10-8 cm = 0.132 nm

3.11 For the simple cubic crystal structure, the value of n in Equation (3.5) is unity since there is only

a single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R.

Therefore, employment of Equation (3.5) yields

ρ=

=

nA

nA

=

VCNA (2R)3N

A

(1 atom/unit cell)(70.4 g/mol)

(2)(1.26 x 10-8 cm) 3 /unit cell(6.023 x 1023 atoms/mol)

[

]

= 7.30 g/cm3

3.12. (a) The volume of the Zr unit cell may be computed using Equation (3.5) as

VC =

nAZr

ρNA

Now, for HCP, n = 6 atoms/unit cell, and for Zr, A

16

Zr

= 91.2 g/mol. Thus,

VC =

(6 atoms/unit cell)(91.2 g/mol)

(6.51 g/cm3 )(6.023 x 1023 atoms/mol)

= 1.396 x 10-22 cm3 /unit cell = 1.396 x 10-28 m3 /unit cell

(b) From the solution to Problem 3.7, since a = 2R, then, for HCP

VC =

3

√ 3a2c

2

but, since c = 1.593a

VC =

3

√ 3(1.593)a3 = 1.396 x 10-22 cm3/unit cell

2

Now, solving for a

(2)(1.396 x 10-22 cm3) 1/3

a=

(3)(

√ 3)(1.593)

= 3.23 x 10-8 cm = 0.323 nm

And finally

c = 1.593a = (1.593)(0.323 nm) = 0.515 nm

3.13 This problem asks that we calculate the theoretical densities of Pb, Cr, Cu, and Co.

3

Since Pb has an FCC crystal structure, n = 4, and V C = 2R

√ 2 . Also, R = 0.175 nm

(1.75 x 10-8 cm) and A Pb = 207.2 g/mol. Employment of Equation (3.5) yields

(

ρ=

)

(4 atoms/unit cell)(207.2 g/mol)

-8

(2)(1.75 x 10 cm)(

√ 2) 3/unit cell(6.023 x 1023 atoms/mol)

[

]

= 11.35 g/cm3

The value given in the table inside the front cover is 11.35 g/cm3 .

Chromium has a BCC crystal structure for which n = 2 and a = 4R/

√ 3; also A Cr = 52.00

g/mol and R = 0.125 nm. Therefore, employment of Equation (3.5) leads to

17

ρ=

(2 atoms/unit cell)(52.00 g/mol)

(4)(1.25 x 10-8 cm) 3

/unit cell(6.023 x 1023 atoms/mol)

3

√

= 7.18 g/cm3

The value given in the table is 7.19 g/cm3 .

Copper has an FCC crystal structure; therefore,

ρ=

(4 atoms/unit cell)(63.55 g/mol)

-8

(2)(1.28 x 10 cm)(

√ 2) 3/unit cell(6.023 x 1023 atoms/mol)

[

]

= 8.89 g/cm3

The value given in the table is 8.94 g/cm3 .

Cobalt has an HCP crystal structure, and from Problem 3.7,

VC =

3

√ 3a2c

2

and, since c = 1.623a and a = 2R = 2(1.25 x 10-8 cm) = 2.50 x 10-8 cm

VC =

(

)

3

√ 3(1.623) 2.50 x 10-8 cm 3

= 6.59 x 10-23 cm3/unit cell

2

Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is

ρ=

=

nACo

VCNA

(6 atoms/unit cell)(58.93 g/mol)

-23

(6.59 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 8.91 g/cm3

18

The value given in the table is 8.9 g/cm3 .

3.14 In order to determine whether Rh has an FCC or BCC crystal structure, we need to compute its

density for each of the crystal structures. For FCC, n = 4, and a = 2R

√ 2. Also, from Figure 2.6,

its atomic weight is 102.91 g/mol. Thus, for FCC

ρ=

=

nARh

(2R√ 2)3NA

(4 atoms/unit cell)(102.91 g/mol)

3

(2)(1.345 x 10-8 cm)(

√ 2) /unit cell(6.023 x 1023 atoms/mol)

[

]

= 12.41 g/cm3

which is the value provided in the problem. Therefore, Rh has an FCC crystal structure.

3.15

For each of these three alloys we need to, by trial and error, calculate the density using

Equation (3.5), and compare it to the value cited in the problem. For SC, BCC, and FCC crystal

structures, the respective values of n are 1, 2, and 4, whereas the expressions for a (since V C =

a3) are 2R, 2R

√ 2, and 4R/√

3.

For alloy A, let us calculate ρ assuming a simple cubic crystal structure.

ρ=

nA A

VCNA

(1 atom/unit cell)(77.4 g/mol)

3

(2)(1.25 x 10-8 cm) /unit cell(6.023 x 1023 atoms/mol)

=

[

]

= 8.22 g/cm3

Therefore, its crystal structure is SC.

For alloy B, let us calculate ρ assuming an FCC crystal structure.

ρ=

(4 atoms/unit cell)(107.6 g/mol)

3

(2)

√ 2(1.33 x 10-8 cm) /unit cell(6.023 x 1023 atoms/mol)

[

]

19

= 13.42 g/cm3

Therefore, its crystal structure is FCC.

For alloy C, let us calculate ρ assuming an SC crystal structure.

ρ=

(1 atom/unit cell)(127.3 g/mol)

3

-8

(2)(1.42 x 10 cm) /unit cell(6.023 x 1023 atoms/mol)

[

]

= 9.23 g/cm3

Therefore, its crystal structure is SC.

3.16 In order to determine the APF for Sn, we need to compute both the unit cell volume (V C ) which

is just the a 2 c product, as well as the total sphere volume (V S ) which is just the product of the

volume of a single sphere and the number of spheres in the unit cell (n). The value of n may be

calculated from Equation (3.5) as

n=

=

ρVCNA

A Sn

(7.30)(5.83)2(3.18)(x 10-24)(6.023 x 1023)

118.69

= 4.00 atoms/unit cell

Therefore

APF =

(4)

VS

VC

(4)

=

(43πR3)

(a)2(c)

[43(π)(0.151)3]

(0.583)2(0.318)

= 0.534

3.17 (a) From the definition of the APF

20

APF =

VS

VC

n

=

(43πR3)

abc

we may solve for the number of atoms per unit cell, n, as

n=

=

(APF)abc

4 3

πR

3

(0.547)(4.79)(7.25)(9.78)(10-24 cm3)

4

π(1.77 x 10-8 cm)3

3

= 8.0 atoms/unit cell

(b) In order to compute the density, we just employ Equation (3.5) as

ρ=

=

nA I

abcNA

(8 atoms/unit cell)(126.91 g/mol)

(4.79)(7.25)(9.78) x 10-24 cm3/unit cell (6.023 x 1023 atoms/mol)

[

]

= 4.96 g/cm3

3. 18 (a) We are asked to calculate the unit cell volume for Ti. From the solution to Problem 3.7

VC = 6R2c

√3

But, c = 1.58a, and a = 2R, or c = 3.16R, and

VC = (6)(3.16)R3

√3

[

]

= (6)(3.16)(

√ 3) 0.1445 x 10-7 cm 3 = 9.91 x 10-23 cm3/unit cell

(b) The density of Ti is determined as follows:

21

ρ=

nATi

VCNA

For HCP, n = 6 atoms/unit cell, and for Ti, A

ρ=

Ti

= 47.88 g/mol. Thus,

(6 atoms/unit cell)(47.88 g/mol)

-23

(9.91 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 4.81 g/cm3

3

The value given in the literature is 4.51 g/cm .

3.19 This problem calls for us to compute the atomic radius for Zn. In order to do this we must use

Equation (3.5), as well as the expression which relates the atomic radius to the unit cell volume

for HCP; from Problem 3.7 it was shown that

VC = 6R2c

√3

In this case c = 1.856(2R).

Making this substitution into the previous equation, and then

solving for R using Equation (3.5) yields

nAZn

1/3

(1.856)(12√ 3)ρNA

R=

=

(6 atoms/unit cell)(65.39 g/mol)

3

23

(1.856)(12√ 3)(7.13 g/cm )(6.023 x 10 atoms/mol)

1/3

= 1.33 x 10-8 cm = 0.133 nm

3.20 This problem asks that we calculate the unit cell volume for Re which has an HCP crystal

structure. In order to do this, it is necessary to use a result of Problem 3.7, that is

VC = 6R2c

√3

The problem states that c = 1.615a, and a = 2R. Therefore

22

VC = (1.615)(12

√ 3)R3

= (1.615)(12

√ 3)(1.37 x 10-8 cm)3 = 8.63 x 10-23 cm3 = 8.63 x 10-2 nm3

3.21 (a) The unit cell shown in the problem belongs to the tetragonal crystal system since a = b =

0.30 nm, c = 0.40 nm, and α = β = γ = 90°.

(b) The crystal structure would be called body-centered tetragonal.

(c) As with BCC n = 2 atoms/unit cell. Also, for this unit cell

VC = (3.0 x 10-8 cm)2(4.0 x 10-8 cm)

= 3.60 x 10-23 cm3/unit cell

Thus,

ρ=

=

nA

VCNA

(2 atoms/unit cell)(141 g/mol)

-23

(3.60 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 13.0 g/cm3

3.22 The unit cell for AuCu3 is to be generated using the software found on the CD-ROM.

3.23 The unit cell for AuCu is to be generated using the software found on the CD-ROM.

3.24 A unit cell for the body-centered orthorhombic crystal structure is presented below.

90

c

90

90

a

b

23

_

3.25 (a) This portion of the problem calls for us to draw a [121] direction within an orthorhombic unit

cell (a ≠ b ≠ c, α = β = γ = 90°). Such a unit cell with its origin positioned at point O is shown

below. We first move along the +x-axis a units (from point O to point A), then parallel to the +yaxis 2b units (from point A to point B). Finally, we proceed parallel to the z-axis -c units (from

_

point B to point C). The [121] direction is the vector from the origin (point O ) to point C as

shown.

z

a

90

c

O

y

90

90

A

x

B

b

C

(b) We are now asked to draw a (210) plane within an orthorhombic unit cell. First remove the

three indices from the parentheses, and take their reciprocals--i.e., 1/2, 1, and ∞. This means

that the plane intercepts the x-axis at a/2, the y-axis at b, and parallels the z-axis. The plane

that satisfies these requirements has been drawn within the orthorhombic unit cell below.

24

PREFACE

This section of instructors materials contains solutions and answers to all

problems and questions that appear in the textbook. My penmanship leaves

something to be desired; therefore, I generated these solutions/answers using

computer software so that the resulting product would be "readable." Furthermore, I

endeavored to provide complete and detailed solutions in order that: (1) the

instructor, without having to take time to solve a problem, will understand what

principles/skills are to be learned by its solution; and (2) to facilitate student

understanding/learning when the solution is posted.

I would recommended that the course instructor consult these

solutions/answers before assigning problems and questions. In doing so, he or she

ensures that the students will be drilled in the intended principles and concepts. In

addition, the instructor may provide appropriate hints for some of the more difficult

problems.

With regard to symbols, in the text material I elected to boldface those symbols

that are italicized in the textbook. Furthermore, I also endeavored to be consistent

relative to symbol style. However, in several instances, symbols that appear in the

textbook were not available, and it was necessary to make appropriate substitutions.

These include the following: the letter a (unit cell edge length, crack length) is used in

place of the cursive a. And Roman F and E replace script F (Faraday's constant in

Chapter 18) and script E (electric field in Chapter 19), respectively.

I have exercised extreme care in designing these problems/questions, and then

in solving them. However, no matter how careful one is with the preparation of a work

such as this, errors will always remain in the final product. Therefore, corrections,

suggestions, and comments from instructors who use the textbook (as well as their

teaching assistants) pertaining to homework problems/solutions are welcomed. These

may be sent to me in care of the publisher.

CHAPTER 2

ATOMIC STRUCTURE AND INTERATOMIC BONDING

PROBLEM SOLUTIONS

2.1 (a) When two or more atoms of an element have different atomic masses, each is termed an

isotope.

(b) The atomic weights of the elements ordinarily are not integers because: (1) the atomic

12

masses of the atoms generally are not integers (except for

C), and (2) the atomic weight is

taken as the weighted average of the atomic masses of an atom's naturally occurring isotopes.

2.2

Atomic mass is the mass of an individual atom, whereas atomic weight is the average

(weighted) of the atomic masses of an atom's naturally occurring isotopes.

2.3 (a) In order to determine the number of grams in one amu of material, appropriate manipulation

of the amu/atom, g/mol, and atom/mol relationships is all that is necessary, as

#g/amu =

1 mol

1 g/mol

6.023 x 1023 atoms 1 amu/atom

(

)

= 1.66 x 10-24 g/amu

(b) Since there are 453.6 g/lbm ,

1 lb-mol = (453.6 g/lbm )(6.023 x 1023 atoms/g-mol)

= 2.73 x 1026 atoms/lb-mol

2.4 (a) Two important quantum-mechanical concepts associated with the Bohr model of the atom

are that electrons are particles moving in discrete orbitals, and electron energy is quantized into

shells.

(b)

Two important refinements resulting from the wave-mechanical atomic model are that

electron position is described in terms of a probability distribution, and electron energy is

quantized into both shells and subshells--each electron is characterized by four quantum

numbers.

1

2.5 The n quantum number designates the electron shell.

The l quantum number designates the electron subshell.

The m quantum number designates the number of electron states in each electron subshell.

l

The m quantum number designates the spin moment on each electron.

s

2.6 For the L state, n = 2, and eight electron states are possible. Possible l values are 0 and 1,

while possible m l values are 0 and ±1. Therefore, for the s states, the quantum numbers are

1

1

1

1

1

200( ) and 200(- ). For the p states, the quantum numbers are 210( ), 210(- ), 211( ), 211(2

2

2

2

2

1

1

1

), 21(-1)( ), and 21(-1)(- ).

2

2

2

For the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2;

1

possible m l values are 0, ±1, and ±2; and possible m s values are ± . Therefore, for the s

2

1

1

1

1

states, the quantum numbers are 300( ), 300(- ), for the p states they are 310( ), 310(- ),

2

2

2

2

311(\F(1,2)), 311(-\F(1,2)), 31(-1)(\F(1,2)), and 31(-1)(-\F(1,2)); for the d states they are

1

1

1

1

1

1

1

1

1

1

320( ), 320(- ), 321( ), 321(- ), 32(-1)( ), 32(-1)(- ), 322( ), 322(- ), 32(-2)( ), and 32(-2)(- ).

2

2

2

2

2

2

2

2

2

2

2.7 The electron configurations of the ions are determined using Table 2.2.

2 2 6 2 6 6

- 1s 2s 2p 3s 3p 3d

3+

2 2 6 2 6 5

Fe

- 1s 2s 2p 3s 3p 3d

+

2 2 6 2 6 10

Cu - 1s 2s 2p 3s 3p 3d

2+

2 2 6 2 6 10 2 6 10 2 6

Ba

- 1s 2s 2p 3s 3p 3d 4s 4p 4d 5s 5p

2 2 6 2 6 10 2 6

Br - 1s 2s 2p 3s 3p 3d 4s 4p

22 2 6 2 6

S - 1s 2s 2p 3s 3p

Fe

2.8 The Cs

+

2+

ion is just a cesium atom that has lost one electron; therefore, it has an electron

configuration the same as xenon (Figure 2.6).

The Br ion is a bromine atom that has acquired one extra electron; therefore, it has an

electron configuration the same as krypton.

2.9 Each of the elements in Group VIIA has five p electrons.

2 2 6 2 6 7 2

2.10 (a) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because

of an incomplete d subshell.

2

2 2 6 2 6

(b) The 1s 2s 2p 3s 3p electron configuration is that of an inert gas because of filled 3s and

3p subshells.

2 2 5

(c) The 1s 2s 2p electron configuration is that of a halogen because it is one electron

deficient from having a filled L shell.

2 2 6 2

(d) The 1s 2s 2p 3s electron configuration is that of an alkaline earth metal because of two s

electrons.

2 2 6 2 6 2 2

(e) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of

an incomplete d subshell.

2 2 6 2 6 1

(f) The 1s 2s 2p 3s 3p 4s electron configuration is that of an alkali metal because of a

single s electron.

2.11 (a) The 4f subshell is being filled for the rare earth series of elements.

(b) The 5f subshell is being filled for the actinide series of elements.

2.12 The attractive force between two ions F A is just the derivative with respect to the interatomic

separation of the attractive energy expression, Equation (2.8), which is just

FA =

dEA

dr

( Ar) = A

d =

dr

r2

The constant A in this expression is defined in footnote 3 on page 21. Since the valences of

the K+ and O2- ions are +1 and -2, respectively, Z1 = 1 and Z 2 = 2, then

FA =

=

(Z1e)(Z2e)

4πε o r2

(1)(2)(1.6 x 10-19 C)2

(4)(π)(8.85 x 10-12 F/m)(1.5 x 10-9 m)2

= 2.05 x 10-10 N

2.13 (a) Differentiation of Equation (2.11) yields

dEN

dr

A

nB

= (1 + 1) - (n + 1) = 0

r

r

3

(b) Now, solving for r (= r )

o

A

nB

= (n + 1)

2

ro ro

or

ro =

(nBA )

1/(1 - n)

(c) Substitution for ro into Equation (2.11) and solving for E (= Eo)

A B

+

ro rn

o

Eo = -

=-

A

+

A 1/(1 - n)

nB

( )

B

A n/(1 - n)

nB

( )

2.14 (a) Curves of E , E , and E are shown on the plot below.

A R

N

2

1

E

R

0

Bonding Energy (eV)

EN

-1

r = 0.28 nm

o

-2

-3

-4

E o = -4.6 eV

-5

EA

-6

-7

0.0

0.2

0.4

0.6

Interatomic Separation (nm)

4

0.8

1.0

(b) From this plot

r = 0.28 nm

o

E = -4.6 eV

o

(c) From Equation (2.11) for E

N

A = 1.436

B = 5.86 x 10

-6

n=9

Thus,

ro =

=

(nBA )

1/(1 - n)

1.436

1/(1 - 9) = 0.279 nm

-6

(9)(5.86 x 10 )

and

Eo= -

1.436

5.86 x 10-6

+

1.436

1.436

1/(1 - 9)

9/(1 - 9)

-6

-6

(9)(5.86 x 10 )

(9)(5.86 x 10 )

= - 4.57 eV

2.15 This problem gives us, for a hypothetical X+ -Y- ion pair, values for ro (0.35 nm), E o (-6.13 eV),

and n (10), and asks that we determine explicit expressions for attractive and repulsive energies

of Equations 2.8 and 2.9. In essence, it is necessary to compute the values of A and B in

these equations. Expressions for r o and E o in terms of n, A , and B were determined in

Problem 2.13, which are as follows:

ro =

Eo = -

(nBA )

1/(1 - n)

A

+

A 1/(1 - n)

nB

( )

B

A n/(1 - n)

nB

( )

Thus, we have two simultaneous equations with two unknowns (viz. A and B). Upon substitution

of values for ro and E o in terms of n, these equations take the forms

5

A

(10B

)

0.35 nm =

-6.13 eV = -

1/(1 - 10)

A

+

A 1/(1 - 10)

10B

( )

B

A 10/(1 - 10)

10B

( )

Simultaneous solution of these two equations leads to A = 2.38 and B = 1.88 x 10-5 . Thus,

Equations (2.8) and (2.9) become

EA = -

ER =

2.38

r

1.88 x 10-5

r10

Of course these expressions are valid for r and E in units of nanometers and electron volts,

respectively.

2.16 (a) Differentiating Equation (2.12) with respect to r yields

dE C De-r/ρ

= dr r2

ρ

At r = ro , dE/dr = 0, and

C De-ro/ρ

2=

ρ

ro

Solving for C and substitution into Equation (2.12) yields an expression for E o as

r

Eo = De-ro/ρ 1 - o

ρ

(b) Now solving for D from Equation (2.12b) above yields

D=

r /ρ

Cρe o

r2o

6

(2.12b)

Substitution of this expression for D into Equation (2.12) yields an expression for Eo as

Eo =

C ρ

- 1

ro ro

2.17 (a) The main differences between the various forms of primary bonding are:

Ionic--there is electrostatic attraction between oppositely charged ions.

Covalent--there is electron sharing between two adjacent atoms such that each atom

assumes a stable electron configuration.

Metallic--the positively charged ion cores are shielded from one another, and also "glued"

together by the sea of valence electrons.

(b) The Pauli exclusion principle states that each electron state can hold no more than two

electrons, which must have opposite spins.

2.18 Covalently bonded materials are less dense than metallic or ionically bonded ones because

covalent bonds are directional in nature whereas metallic and ionic are not; when bonds are

directional, the atoms cannot pack together in as dense a manner, yielding a lower mass

density.

2.19 The percent ionic character is a function of the electron negativities of the ions X A and X B

according to Equation (2.10). The electronegativities of the elements are found in Figure 2.7.

For TiO2, X Ti = 1.5 and X O = 3.5, and therefore,

[

%IC = 1 - e(-0.25)(3.5 - 1.5)

2

] x 100 = 63.2%

For ZnTe, X Zn = 1.6 and X Te = 2.1, and therefore,

[

%IC = 1 - e(-0.25)(2.1 - 1.6)

2

] x 100 = 6.1%

For CsCl, X Cs = 0.7 and X Cl = 3.0, and therefore,

[

%IC = 1 - e(-0.25)(3.0 - 0.7)

For InSb, X In = 1.7 and X Sb = 1.9, and therefore,

7

2

] x 100 = 73.4%

[

%IC = 1 - e(-0.25)(1.9 - 1.7)

2

] x 100 = 1.0%

For MgCl2, X Mg = 1.2 and X Cl = 3.0, and therefore,

[

%IC = 1 - e(-0.25)(3.0 - 1.2)

2

] x 100 = 55.5%

2.20 Below is plotted the bonding energy versus melting temperature for these four metals. From

this plot, the bonding energy for copper (melting temperature of 1084°C) should be

approximately 3.6 eV. The experimental value is 3.5 eV.

Bonding Energy (eV)

10

W

8

6

4

Fe

3.6 eV

Al

2

0

-1000

Hg

0

1000

2000

3000

4000

Melting Temperature (C)

2 2

2.21 For germanium, having the valence electron structure 4s 4p , N' = 4; thus, there are 8 - N' = 4

covalent bonds per atom.

2 3

For phosphorus, having the valence electron structure 3s 3p , N' = 5; thus, there are 8

- N' = 3 covalent bonds per atom.

2 4

For selenium, having the valence electron structure 4s 4p , N' = 6; thus, there are 8 N' = 2 covalent bonds per atom.

2 5

For chlorine, having the valence electron structure 3s 3p , N' = 7; thus, there is 8 - N' =

1 covalent bond per atom.

2.22 For brass, the bonding is metallic since it is a metal alloy.

For rubber, the bonding is covalent with some van der Waals. (Rubber is composed

primarily of carbon and hydrogen atoms.)

8

For BaS, the bonding is predominantly ionic (but with some covalent character) on the

basis of the relative positions of Ba and S in the periodic table.

For solid xenon, the bonding is van der Waals since xenon is an inert gas.

For bronze, the bonding is metallic since it is a metal alloy (composed of copper and tin).

For nylon, the bonding is covalent with perhaps some van der Waals.

(Nylon is

composed primarily of carbon and hydrogen.)

For AlP the bonding is predominantly covalent (but with some ionic character) on the

basis of the relative positions of Al and P in the periodic table.

2.23 The intermolecular bonding for HF is hydrogen, whereas for HCl, the intermolecular bonding is

van der Waals. Since the hydrogen bond is stronger than van der Waals, HF will have a higher

melting temperature.

2.24 The geometry of the H O molecules, which are hydrogen bonded to one another, is more

2

restricted in the solid phase than for the liquid. This results in a more open molecular structure in

the solid, and a less dense solid phase.

9

CHAPTER 3

THE STRUCTURE OF CRYSTALLINE SOLIDS

PROBLEM SOLUTIONS

3.1 Atomic structure relates to the number of protons and neutrons in the nucleus of an atom, as

well as the number and probability distributions of the constituent electrons. On the other hand,

crystal structure pertains to the arrangement of atoms in the crystalline solid material.

3.2 A crystal structure is described by both the geometry of, and atomic arrangements within, the

unit cell, whereas a crystal system is described only in terms of the unit cell geometry. For

example, face-centered cubic and body-centered cubic are crystal structures that belong to the

cubic crystal system.

3.3 For this problem, we are asked to calculate the volume of a unit cell of aluminum. Aluminum

has an FCC crystal structure (Table 3.1). The FCC unit cell volume may be computed from

Equation (3.4) as

√ 2 = (16)(0.143 x 10-9 m)3√ 2 = 6.62 x 10-29 m3

VC = 16R3

3.4 This problem calls for a demonstration of the relationship a = 4R

√ 3 for BCC. Consider the BCC

unit cell shown below

a

Q

a

P

N

O

a

Using the triangle NOP

10

__

2

(NP) = a2 + a2 = 2a2

And then for triangle NPQ,

__

__

__

(NQ )2 = (QP )2 + (NP )2

__

__

But NQ = 4R, R being the atomic radius. Also, QP = a. Therefore,

(4R)2 = a2 + 2a2, or

a=

4R

3

√

3.5 We are asked to show that the ideal c/a ratio for HCP is 1.633. A sketch of one-third of an HCP

unit cell is shown below.

a

c

M

L

J

K

a

Consider the tetrahedron labeled as JKLM, which is reconstructed as

11

M

L

H

J

K

__

The atom at point M is midway between the top and bottom faces of the unit cell--that is M H =

c/2. And, since atoms at points J, K, and M, all touch one another,

__ __

JM = JK = 2R = a

where R is the atomic radius. Furthermore, from triangle JHM,

__

__

__

__

(c2)2

(JM )2 = ( JH )2 + (MH)2, or

a2 = ( JH )2 +

__

Now, we can determine the JH length by consideration of triangle JKL, which is an equilateral

triangle,

L

J

30

H

a/2

K

cos 30° =

a/2

√ 3 , and

=

JH

2

__

JH =

12

a

3

√

__

Substituting this value for JH in the above expression yields

a2 =

2

2

a 2 + c 2 = a + c

2

3

4

3

√

()

and, solving for c/a

c

=

a

√ 83 = 1.633

3.6 We are asked to show that the atomic packing factor for BCC is 0.68. The atomic packing factor

is defined as the ratio of sphere volume to the total unit cell volume, or

APF =

VS

VC

Since there are two spheres associated with each unit cell for BCC

4πR3 8πR 3

=

3

3

V S = 2(sphere volume) = 2

Also, the unit cell has cubic symmetry, that is V

C

3

= a . But a depends on R according to

Equation (3.3), and

VC =

4R 3

3

√

=

64R 3

3√

3

Thus,

APF =

8πR 3 /3

= 0.68

64R 3 /3

√3

3.7 This problem calls for a demonstration that the APF for HCP is 0.74. Again, the APF is just the

total sphere-unit cell volume ratio. For HCP, there are the equivalent of six spheres per unit cell,

and thus

13

4πR3

= 8πR 3

3

V S = 6

Now, the unit cell volume is just the product of the base area times the cell height, c. This base

area is just three times the area of the parallelepiped ACDE shown below.

D

C

a = 2R

30

60

E

A

B

a = 2R

a = 2R

__

__

__

The area of ACDE is just the length of CD times the height BC. But CD is just a or 2R, and

__

BC = 2R cos(30°) =

2R

√3

2

Thus, the base area is just

__ __

2R√ 3

= 6R2

√3

2

AREA = (3)(CD )(BC ) = (3)(2R)

and since c = 1.633a = 2R(1.633)

VC = (AREA)(c) = 6R2c

√ 3 = (6R2√ 3)(2)(1.633)R = 12√ 3(1.633)R3

Thus,

APF =

VS

VC

=

8πR 3

12 √

3(1.633)R3

= 0.74

3.8 This problem calls for a computation of the density of iron. According to Equation (3.5)

14

ρ=

nAFe

VCNA

For BCC, n = 2 atoms/unit cell, and

VC =

4R 3

3

√

Thus,

ρ=

(2 atoms/unit cell)(55.9 g/mol)

(4)(0.124 x 10-7 cm)3/

√ 3 3/(unit cell)(6.023 x 1023 atoms/mol)

[

]

= 7.90 g/cm3

3

The value given inside the front cover is 7.87 g/cm .

3.9 We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal

structure. For FCC, n = 4 atoms/unit cell, and V = 16R3

√ 2 [Equation (3.4)]. Now,

C

ρ=

nAIr

VCNA

And solving for R from the above two expressions yields

16ρNA√ 2

R=

nAIr

1/3

(4 atoms/unit cell)(192.2 g/mol)

=

3

23

(√ 2)(16)(22.4 g/cm )(6.023 x 10 atoms/mol)

1/3

= 1.36 x 10-8 cm = 0.136 nm

3.10

This problem asks for us to calculate the radius of a vanadium atom. For BCC, n = 2

atoms/unit cell, and

15

VC =

4R 3

3

√

=

64R 3

3√

3

Since,

ρ=

nA V

VCNA

and solving for R

R=

3√

3nA V 1/3

64ρNA

(3√ 3)(2 atoms/unit cell)(50.9 g/mol) 1/3

=

(64)(5.96 g/cm3)(6.023 x 1023 atoms/mol)

= 1.32 x 10-8 cm = 0.132 nm

3.11 For the simple cubic crystal structure, the value of n in Equation (3.5) is unity since there is only

a single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R.

Therefore, employment of Equation (3.5) yields

ρ=

=

nA

nA

=

VCNA (2R)3N

A

(1 atom/unit cell)(70.4 g/mol)

(2)(1.26 x 10-8 cm) 3 /unit cell(6.023 x 1023 atoms/mol)

[

]

= 7.30 g/cm3

3.12. (a) The volume of the Zr unit cell may be computed using Equation (3.5) as

VC =

nAZr

ρNA

Now, for HCP, n = 6 atoms/unit cell, and for Zr, A

16

Zr

= 91.2 g/mol. Thus,

VC =

(6 atoms/unit cell)(91.2 g/mol)

(6.51 g/cm3 )(6.023 x 1023 atoms/mol)

= 1.396 x 10-22 cm3 /unit cell = 1.396 x 10-28 m3 /unit cell

(b) From the solution to Problem 3.7, since a = 2R, then, for HCP

VC =

3

√ 3a2c

2

but, since c = 1.593a

VC =

3

√ 3(1.593)a3 = 1.396 x 10-22 cm3/unit cell

2

Now, solving for a

(2)(1.396 x 10-22 cm3) 1/3

a=

(3)(

√ 3)(1.593)

= 3.23 x 10-8 cm = 0.323 nm

And finally

c = 1.593a = (1.593)(0.323 nm) = 0.515 nm

3.13 This problem asks that we calculate the theoretical densities of Pb, Cr, Cu, and Co.

3

Since Pb has an FCC crystal structure, n = 4, and V C = 2R

√ 2 . Also, R = 0.175 nm

(1.75 x 10-8 cm) and A Pb = 207.2 g/mol. Employment of Equation (3.5) yields

(

ρ=

)

(4 atoms/unit cell)(207.2 g/mol)

-8

(2)(1.75 x 10 cm)(

√ 2) 3/unit cell(6.023 x 1023 atoms/mol)

[

]

= 11.35 g/cm3

The value given in the table inside the front cover is 11.35 g/cm3 .

Chromium has a BCC crystal structure for which n = 2 and a = 4R/

√ 3; also A Cr = 52.00

g/mol and R = 0.125 nm. Therefore, employment of Equation (3.5) leads to

17

ρ=

(2 atoms/unit cell)(52.00 g/mol)

(4)(1.25 x 10-8 cm) 3

/unit cell(6.023 x 1023 atoms/mol)

3

√

= 7.18 g/cm3

The value given in the table is 7.19 g/cm3 .

Copper has an FCC crystal structure; therefore,

ρ=

(4 atoms/unit cell)(63.55 g/mol)

-8

(2)(1.28 x 10 cm)(

√ 2) 3/unit cell(6.023 x 1023 atoms/mol)

[

]

= 8.89 g/cm3

The value given in the table is 8.94 g/cm3 .

Cobalt has an HCP crystal structure, and from Problem 3.7,

VC =

3

√ 3a2c

2

and, since c = 1.623a and a = 2R = 2(1.25 x 10-8 cm) = 2.50 x 10-8 cm

VC =

(

)

3

√ 3(1.623) 2.50 x 10-8 cm 3

= 6.59 x 10-23 cm3/unit cell

2

Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is

ρ=

=

nACo

VCNA

(6 atoms/unit cell)(58.93 g/mol)

-23

(6.59 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 8.91 g/cm3

18

The value given in the table is 8.9 g/cm3 .

3.14 In order to determine whether Rh has an FCC or BCC crystal structure, we need to compute its

density for each of the crystal structures. For FCC, n = 4, and a = 2R

√ 2. Also, from Figure 2.6,

its atomic weight is 102.91 g/mol. Thus, for FCC

ρ=

=

nARh

(2R√ 2)3NA

(4 atoms/unit cell)(102.91 g/mol)

3

(2)(1.345 x 10-8 cm)(

√ 2) /unit cell(6.023 x 1023 atoms/mol)

[

]

= 12.41 g/cm3

which is the value provided in the problem. Therefore, Rh has an FCC crystal structure.

3.15

For each of these three alloys we need to, by trial and error, calculate the density using

Equation (3.5), and compare it to the value cited in the problem. For SC, BCC, and FCC crystal

structures, the respective values of n are 1, 2, and 4, whereas the expressions for a (since V C =

a3) are 2R, 2R

√ 2, and 4R/√

3.

For alloy A, let us calculate ρ assuming a simple cubic crystal structure.

ρ=

nA A

VCNA

(1 atom/unit cell)(77.4 g/mol)

3

(2)(1.25 x 10-8 cm) /unit cell(6.023 x 1023 atoms/mol)

=

[

]

= 8.22 g/cm3

Therefore, its crystal structure is SC.

For alloy B, let us calculate ρ assuming an FCC crystal structure.

ρ=

(4 atoms/unit cell)(107.6 g/mol)

3

(2)

√ 2(1.33 x 10-8 cm) /unit cell(6.023 x 1023 atoms/mol)

[

]

19

= 13.42 g/cm3

Therefore, its crystal structure is FCC.

For alloy C, let us calculate ρ assuming an SC crystal structure.

ρ=

(1 atom/unit cell)(127.3 g/mol)

3

-8

(2)(1.42 x 10 cm) /unit cell(6.023 x 1023 atoms/mol)

[

]

= 9.23 g/cm3

Therefore, its crystal structure is SC.

3.16 In order to determine the APF for Sn, we need to compute both the unit cell volume (V C ) which

is just the a 2 c product, as well as the total sphere volume (V S ) which is just the product of the

volume of a single sphere and the number of spheres in the unit cell (n). The value of n may be

calculated from Equation (3.5) as

n=

=

ρVCNA

A Sn

(7.30)(5.83)2(3.18)(x 10-24)(6.023 x 1023)

118.69

= 4.00 atoms/unit cell

Therefore

APF =

(4)

VS

VC

(4)

=

(43πR3)

(a)2(c)

[43(π)(0.151)3]

(0.583)2(0.318)

= 0.534

3.17 (a) From the definition of the APF

20

APF =

VS

VC

n

=

(43πR3)

abc

we may solve for the number of atoms per unit cell, n, as

n=

=

(APF)abc

4 3

πR

3

(0.547)(4.79)(7.25)(9.78)(10-24 cm3)

4

π(1.77 x 10-8 cm)3

3

= 8.0 atoms/unit cell

(b) In order to compute the density, we just employ Equation (3.5) as

ρ=

=

nA I

abcNA

(8 atoms/unit cell)(126.91 g/mol)

(4.79)(7.25)(9.78) x 10-24 cm3/unit cell (6.023 x 1023 atoms/mol)

[

]

= 4.96 g/cm3

3. 18 (a) We are asked to calculate the unit cell volume for Ti. From the solution to Problem 3.7

VC = 6R2c

√3

But, c = 1.58a, and a = 2R, or c = 3.16R, and

VC = (6)(3.16)R3

√3

[

]

= (6)(3.16)(

√ 3) 0.1445 x 10-7 cm 3 = 9.91 x 10-23 cm3/unit cell

(b) The density of Ti is determined as follows:

21

ρ=

nATi

VCNA

For HCP, n = 6 atoms/unit cell, and for Ti, A

ρ=

Ti

= 47.88 g/mol. Thus,

(6 atoms/unit cell)(47.88 g/mol)

-23

(9.91 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 4.81 g/cm3

3

The value given in the literature is 4.51 g/cm .

3.19 This problem calls for us to compute the atomic radius for Zn. In order to do this we must use

Equation (3.5), as well as the expression which relates the atomic radius to the unit cell volume

for HCP; from Problem 3.7 it was shown that

VC = 6R2c

√3

In this case c = 1.856(2R).

Making this substitution into the previous equation, and then

solving for R using Equation (3.5) yields

nAZn

1/3

(1.856)(12√ 3)ρNA

R=

=

(6 atoms/unit cell)(65.39 g/mol)

3

23

(1.856)(12√ 3)(7.13 g/cm )(6.023 x 10 atoms/mol)

1/3

= 1.33 x 10-8 cm = 0.133 nm

3.20 This problem asks that we calculate the unit cell volume for Re which has an HCP crystal

structure. In order to do this, it is necessary to use a result of Problem 3.7, that is

VC = 6R2c

√3

The problem states that c = 1.615a, and a = 2R. Therefore

22

VC = (1.615)(12

√ 3)R3

= (1.615)(12

√ 3)(1.37 x 10-8 cm)3 = 8.63 x 10-23 cm3 = 8.63 x 10-2 nm3

3.21 (a) The unit cell shown in the problem belongs to the tetragonal crystal system since a = b =

0.30 nm, c = 0.40 nm, and α = β = γ = 90°.

(b) The crystal structure would be called body-centered tetragonal.

(c) As with BCC n = 2 atoms/unit cell. Also, for this unit cell

VC = (3.0 x 10-8 cm)2(4.0 x 10-8 cm)

= 3.60 x 10-23 cm3/unit cell

Thus,

ρ=

=

nA

VCNA

(2 atoms/unit cell)(141 g/mol)

-23

(3.60 x 10

cm3/unit cell)(6.023 x 1023 atoms/mol)

= 13.0 g/cm3

3.22 The unit cell for AuCu3 is to be generated using the software found on the CD-ROM.

3.23 The unit cell for AuCu is to be generated using the software found on the CD-ROM.

3.24 A unit cell for the body-centered orthorhombic crystal structure is presented below.

90

c

90

90

a

b

23

_

3.25 (a) This portion of the problem calls for us to draw a [121] direction within an orthorhombic unit

cell (a ≠ b ≠ c, α = β = γ = 90°). Such a unit cell with its origin positioned at point O is shown

below. We first move along the +x-axis a units (from point O to point A), then parallel to the +yaxis 2b units (from point A to point B). Finally, we proceed parallel to the z-axis -c units (from

_

point B to point C). The [121] direction is the vector from the origin (point O ) to point C as

shown.

z

a

90

c

O

y

90

90

A

x

B

b

C

(b) We are now asked to draw a (210) plane within an orthorhombic unit cell. First remove the

three indices from the parentheses, and take their reciprocals--i.e., 1/2, 1, and ∞. This means

that the plane intercepts the x-axis at a/2, the y-axis at b, and parallels the z-axis. The plane

that satisfies these requirements has been drawn within the orthorhombic unit cell below.

24

## SOLUTIONS MANUAL Communication Systems Engineering Second EditionJohn G. Proakis Masoud ppt

## SOLUTIONS MANUAL Communication Systems Engineering Second EditionJohn G. Proakis ppt

## unit operation of chemical engineering 7th ed, solutions manual

## ceramic materials - science and engineering

## materials science and engineering an introduction, 7th edition

## nanoporous materials science and engineering (series on chemical engineering)

## supercritical fluid technology in materials science and engineering

## introduction chemical engineering thermodynamics 7ed solutions manual

## Biomedical Engineering Trends in Materials Science Part 1 doc

## Biomedical Engineering Trends in Materials Science Part 3 pdf

Tài liệu liên quan